Download presentation

Presentation is loading. Please wait.

1
**Chapter 3: The Structure of Crystalline Solids**

ISSUES TO ADDRESS... • How do atoms assemble into solid structures? • How does the density of a material depend on its structure? • When do material properties vary with the sample (i.e., part) orientation?

2
**Energy and Packing • Non dense, random packing**

typical neighbor bond length bond energy • Dense, ordered packing Energy r typical neighbor bond length bond energy Dense, ordered packed structures tend to have lower energies.

3
**Materials and Packing Si Oxygen Crystalline materials...**

• atoms pack in periodic, 3D arrays • typical of: -metals -many ceramics -some polymers crystalline SiO2 Adapted from Fig. 3.23(a), Callister & Rethwisch 8e. Si Oxygen Noncrystalline materials... • atoms have no periodic packing • occurs for: -complex structures -rapid cooling "Amorphous" = Noncrystalline noncrystalline SiO2 Adapted from Fig. 3.23(b), Callister & Rethwisch 8e.

4
** Metallic Crystal Structures**

How can we stack metal atoms to minimize empty space? 2-dimensions vs. Now stack these 2-D layers to make 3-D structures

5
**Metallic Crystal Structures**

• Tend to be densely packed. • Reasons for dense packing: - Typically, only one element is present, so all atomic radii are the same. - Metallic bonding is not directional. - Nearest neighbor distances tend to be small in order to lower bond energy. - Electron cloud shields cores from each other • Have the simplest crystal structures. We will examine three such structures...

6
**Simple Cubic Structure (SC)**

• Rare due to low packing density (only Po has this structure) • Close-packed directions are cube edges. • Coordination # = 6 (# nearest neighbors) Click once on image to start animation (Courtesy P.M. Anderson)

7
**Atomic Packing Factor (APF)**

Volume of atoms in unit cell* APF = Volume of unit cell *assume hard spheres • APF for a simple cubic structure = 0.52 Adapted from Fig. 3.24, Callister & Rethwisch 8e. close-packed directions a R=0.5a contains 8 x 1/8 = 1 atom/unit cell atom volume atoms unit cell 4 3 p (0.5a) 1 APF = 3 a unit cell volume

8
**Body Centered Cubic Structure (BCC)**

• Atoms touch each other along cube diagonals. --Note: All atoms are identical; the center atom is shaded differently only for ease of viewing. ex: Cr, W, Fe (), Tantalum, Molybdenum • Coordination # = 8 Adapted from Fig. 3.2, Callister & Rethwisch 8e. Click once on image to start animation (Courtesy P.M. Anderson) 2 atoms/unit cell: 1 center + 8 corners x 1/8

9
**Atomic Packing Factor: BCC**

• APF for a body-centered cubic structure = 0.68 a R a 3 a a 2 length = 4R = Close-packed directions: 3 a Adapted from Fig. 3.2(a), Callister & Rethwisch 8e. APF = 4 3 p ( a/4 ) 2 atoms unit cell atom volume a

10
**Face Centered Cubic Structure (FCC)**

• Atoms touch each other along face diagonals. --Note: All atoms are identical; the face-centered atoms are shaded differently only for ease of viewing. ex: Al, Cu, Au, Pb, Ni, Pt, Ag • Coordination # = 12 Adapted from Fig. 3.1, Callister & Rethwisch 8e. Click once on image to start animation 4 atoms/unit cell: 6 face x 1/2 + 8 corners x 1/8 (Courtesy P.M. Anderson)

11
**Atomic Packing Factor: FCC**

• APF for a face-centered cubic structure = 0.74 a 2 a maximum achievable APF Close-packed directions: length = 4R = 2 a Unit cell contains: 6 x 1/2 + 8 x 1/8 = 4 atoms/unit cell Adapted from Fig. 3.1(a), Callister & Rethwisch 8e. APF = 4 3 p ( 2 a/4 ) atoms unit cell atom volume a

12
**FCC Stacking Sequence • ABCABC... Stacking Sequence • 2D Projection**

A sites B C sites A B sites C A C A A B C • FCC Unit Cell

13
**Hexagonal Close-Packed Structure (HCP)**

• ABAB... Stacking Sequence • 3D Projection • 2D Projection c a A sites B sites Bottom layer Middle layer Top layer Adapted from Fig. 3.3(a), Callister & Rethwisch 8e. • Coordination # = 12 6 atoms/unit cell • APF = 0.74 ex: Cd, Mg, Ti, Zn • c/a = 1.633

14
**Theoretical Density, r Density = = n A = VC NA**

Cell Unit of Volume Total in Atoms Mass Density = = VC NA n A = where n = number of atoms/unit cell A = atomic weight VC = Volume of unit cell = a3 for cubic NA = Avogadro’s number = x 1023 atoms/mol

15
**Theoretical Density, r = a R Ex: Cr (BCC) A = 52.00 g/mol**

R = nm n = 2 atoms/unit cell a = 4R/ 3 = nm Adapted from Fig. 3.2(a), Callister & Rethwisch 8e. = a3 52.00 2 atoms unit cell mol g volume 6.022 x 1023 theoretical = 7.18 g/cm3 ractual = 7.19 g/cm3

16
**Densities of Material Classes**

In general Graphite/ r metals r ceramics r polymers Metals/ Composites/ > > Ceramics/ Polymers Alloys fibers Semicond 30 Why? B ased on data in Table B1, Callister Metals have... • close-packing (metallic bonding) • often large atomic masses 2 Magnesium Aluminum Steels Titanium Cu,Ni Tin, Zinc Silver, Mo Tantalum Gold, W Platinum *GFRE, CFRE, & AFRE are Glass, Carbon, & Aramid Fiber-Reinforced Epoxy composites (values based on 60% volume fraction of aligned fibers 10 in an epoxy matrix). G raphite Silicon Glass - soda Concrete Si nitride Diamond Al oxide Zirconia Ceramics have... • less dense packing • often lighter elements 5 3 4 (g/cm ) 3 Wood AFRE * CFRE GFRE* Glass fibers Carbon fibers A ramid fibers H DPE, PS PP, LDPE PC PTFE PET PVC Silicone Polymers have... • low packing density (often amorphous) • lighter elements (C,H,O) r 2 1 Composites have... • intermediate values 0.5 0.4 0.3 Data from Table B.1, Callister & Rethwisch, 8e.

17
**Crystals as Building Blocks**

• Some engineering applications require single crystals: -- diamond single crystals for abrasives -- turbine blades Fig. 8.33(c), Callister & Rethwisch 8e. (Fig. 8.33(c) courtesy of Pratt and Whitney). (Courtesy Martin Deakins, GE Superabrasives, Worthington, OH. Used with permission.) • Properties of crystalline materials often related to crystal structure. -- Ex: Quartz fractures more easily along some crystal planes than others. (Courtesy P.M. Anderson)

18
**Polycrystals Anisotropic**

• Most engineering materials are polycrystals. Adapted from Fig. K, color inset pages of Callister 5e. (Fig. K is courtesy of Paul E. Danielson, Teledyne Wah Chang Albany) 1 mm Isotropic • Nb-Hf-W plate with an electron beam weld. • Each "grain" is a single crystal. • If grains are randomly oriented, overall component properties are not directional. • Grain sizes typically range from 1 nm to 2 cm (i.e., from a few to millions of atomic layers).

19
**Single vs Polycrystals**

E (diagonal) = 273 GPa E (edge) = 125 GPa • Single Crystals -Properties vary with direction: anisotropic. Data from Table 3.3, Callister & Rethwisch 8e. (Source of data is R.W. Hertzberg, Deformation and Fracture Mechanics of Engineering Materials, 3rd ed., John Wiley and Sons, 1989.) -Example: the modulus of elasticity (E) in BCC iron: • Polycrystals -Properties may/may not vary with direction. -If grains are randomly oriented: isotropic. (Epoly iron = 210 GPa) -If grains are textured, anisotropic. 200 mm Adapted from Fig. 4.14(b), Callister & Rethwisch 8e. (Fig. 4.14(b) is courtesy of L.C. Smith and C. Brady, the National Bureau of Standards, Washington, DC [now the National Institute of Standards and Technology, Gaithersburg, MD].)

20
Polymorphism Two or more distinct crystal structures for the same material (allotropy/polymorphism) titanium , -Ti carbon diamond, graphite BCC FCC 1538ºC 1394ºC 912ºC -Fe -Fe -Fe liquid iron system

21
Crystal Systems Unit cell: smallest repetitive volume which contains the complete lattice pattern of a crystal. Fig. 3.4, Callister & Rethwisch 8e. 7 crystal systems 14 crystal lattices a, b, and c are the lattice constants

22
**Point Coordinates z Point coordinates for unit cell center are c**

x y a b c 000 111 Point coordinates for unit cell center are a/2, b/2, c/ ½ ½ ½ Point coordinates for unit cell corner are 111 Translation: integer multiple of lattice constants identical position in another unit cell z 2c y b b

23
**Crystallographic Directions**

z pt. 2 head Example 2: pt. 1 x1 = a, y1 = b/2, z1 = 0 pt. 2 x2 = -a, y2 = b, z2 = c y pt. 1: tail x => -2, 1/2, 1 Multiplying by 2 to eliminate the fraction -4, 1, 2 where the overbar represents a negative index [ 412 ] => families of directions <uvw>

24
**Crystallographic Directions**

z Algorithm 1. Vector repositioned (if necessary) to pass through origin. 2. Read off projections in terms of unit cell dimensions a, b, and c 3. Adjust to smallest integer values 4. Enclose in square brackets, no commas [uvw] y x ex: 1, 0, ½ Lecture 2 ended here => 2, 0, 1 => [ 201 ] -1, 1, 1 where overbar represents a negative index [ 111 ] => families of directions <uvw>

25
**Linear Density 3.5 nm a 2 LD = Linear Density of Atoms LD = [110]**

Number of atoms Unit length of direction vector a [110] ex: linear density of Al in [110] direction a = nm # atoms length 1 3.5 nm a 2 LD - = Adapted from Fig. 3.1(a), Callister & Rethwisch 8e.

26
**HCP Crystallographic Directions**

- a3 a1 a2 z Algorithm 1. Vector repositioned (if necessary) to pass through origin. 2. Read off projections in terms of unit cell dimensions a1, a2, a3, or c 3. Adjust to smallest integer values 4. Enclose in square brackets, no commas [uvtw] dashed red lines indicate projections onto a1 and a2 axes a1 a2 a3 -a3 2 a 1 Adapted from Fig. 3.8(a), Callister & Rethwisch 8e. [ 1120 ] ex: ½, ½, -1, =>

27
**HCP Crystallographic Directions**

Hexagonal Crystals 4 parameter Miller-Bravais lattice coordinates are related to the direction indices (i.e., u'v'w') as follows. Fig. 3.8(a), Callister & Rethwisch 8e. - a3 a1 a2 z = ' w t v u ) ( + - 2 3 1 ] uvtw [

28
**Crystallographic Planes**

Adapted from Fig. 3.10, Callister & Rethwisch 8e.

29
**Crystallographic Planes**

Miller Indices: Reciprocals of the (three) axial intercepts for a plane, cleared of fractions & common multiples. All parallel planes have same Miller indices. Algorithm 1. Read off intercepts of plane with axes in terms of a, b, c 2. Take reciprocals of intercepts 3. Reduce to smallest integer values 4. Enclose in parentheses, no commas i.e., (hkl)

30
**Crystallographic Planes**

z x y a b c example a b c Intercepts Reciprocals 1/ / / Reduction Miller Indices (110) example a b c z x y a b c Intercepts 1/ Reciprocals 1/½ 1/ 1/ Reduction Miller Indices (100)

31
**Crystallographic Planes**

z x y a b c example a b c Intercepts 1/ /4 Reciprocals 1/½ 1/ /¾ /3 Reduction Miller Indices (634) (001) (010), Family of Planes {hkl} (100), (001), Ex: {100} = (100),

32
**Crystallographic Planes (HCP)**

In hexagonal unit cells the same idea is used a2 a3 a1 z example a a a c Intercepts -1 1 Reciprocals / -1 1 Reduction -1 1 Miller-Bravais Indices (1011) Adapted from Fig. 3.8(b), Callister & Rethwisch 8e.

33
**Crystallographic Planes**

We want to examine the atomic packing of crystallographic planes Iron foil can be used as a catalyst. The atomic packing of the exposed planes is important. Draw (100) and (111) crystallographic planes for Fe. b) Calculate the planar density for each of these planes.

34
**Virtual Materials Science & Engineering (VMSE)**

• VMSE is a tool to visualize materials science topics such as crystallography and polymer structures in three dimensions • Available in Student Companion Site at and in WileyPLUS

35
**VMSE: Metallic Crystal Structures & Crystallography Module**

• VMSE allows you to view crystal structures, directions, planes, etc. and manipulate them in three dimensions

36
**Unit Cells for Metals FCC Structure HCP Structure**

• VMSE allows you to view the unit cells and manipulate them in three dimensions • Below are examples of actual VMSE screen shots FCC Structure HCP Structure

37
**VMSE: Crystallographic Planes Exercises**

Additional practice on indexing crystallographic planes

38
**Planar Density of (100) Iron**

Solution: At T < 912ºC iron has the BCC structure. 2D repeat unit R 3 4 a = (100) Radius of iron R = nm Adapted from Fig. 3.2(c), Callister & Rethwisch 8e. = Planar Density = a 2 1 atoms 2D repeat unit nm2 12.1 m2 = 1.2 x 1019 R 3 4 area

39
**Planar Density of (111) Iron**

Solution (cont): (111) plane 1 atom in plane/ unit surface cell 2 a atoms in plane atoms above plane atoms below plane 2D repeat unit 3 h = a 2 3 2 R 16 4 a ah area = ø ö ç è æ 1 = nm2 atoms 7.0 m2 0.70 x 1019 3 2 R 16 Planar Density = 2D repeat unit area

40
**VMSE Planar Atomic Arrangements**

• VMSE allows you to view planar arrangements and rotate them in 3 dimensions BCC (110) Plane

41
X-Ray Diffraction Diffraction gratings must have spacings comparable to the wavelength of diffracted radiation. Can’t resolve spacings Spacing is the distance between parallel planes of atoms.

42
**X-Rays to Determine Crystal Structure**

• Incoming X-rays diffract from crystal planes. Adapted from Fig. 3.20, Callister & Rethwisch 8e. reflections must be in phase for a detectable signal spacing between planes d incoming X-rays outgoing X-rays detector q l extra distance travelled by wave “2” “1” “2” X-ray intensity (from detector) q c d = n l 2 sin Measurement of critical angle, qc, allows computation of planar spacing, d.

43
**X-Ray Diffraction Pattern**

z x y a b c z x y a b c z x y a b c (110) (211) Intensity (relative) (200) Diffraction angle 2q Diffraction pattern for polycrystalline a-iron (BCC) Adapted from Fig. 3.22, Callister 8e.

44
**SUMMARY • Atoms may assemble into crystalline or amorphous structures.**

• Common metallic crystal structures are FCC, BCC, and HCP. Coordination number and atomic packing factor are the same for both FCC and HCP crystal structures. • We can predict the density of a material, provided we know the atomic weight, atomic radius, and crystal geometry (e.g., FCC, BCC, HCP). • Crystallographic points, directions and planes are specified in terms of indexing schemes. Crystallographic directions and planes are related to atomic linear densities and planar densities.

45
**SUMMARY • Materials can be single crystals or polycrystalline.**

Material properties generally vary with single crystal orientation (i.e., they are anisotropic), but are generally non-directional (i.e., they are isotropic) in polycrystals with randomly oriented grains. • Some materials can have more than one crystal structure. This is referred to as polymorphism (or allotropy). • X-ray diffraction is used for crystal structure and interplanar spacing determinations.

46
ANNOUNCEMENTS Reading: Core Problems: Self-help Problems:

Similar presentations

© 2017 SlidePlayer.com Inc.

All rights reserved.

Ads by Google